Effect of utilizing unground and ground normal and black rice husk ash on the mechanical and durability properties of high-strength concrete
Page content transcription ( If your browser does not render page correctly, please read the page content below )
Sådhanå (2018) 43:22 Ó Indian Academy of Sciences https://doi.org/10.1007/s12046-018-0795-0 Sadhana(0123456789().,-volV)FT3 ](0123456789().,-volV) Effect of utilizing unground and ground normal and black rice husk ash on the mechanical and durability properties of high-strength concrete SYAMSUL BAHRI1,2, H B MAHMUD1,* and PAYAM SHAFIGH3 1 Department of Civil Engineering, Faculty of Engineering, University of Malaya, 50603 Kuala Lumpur, Malaysia 2 Department of Civil Engineering, Lhokseumawe State Polytechnic, Lhokseumawe, Indonesia 3 Department of Building Surveying, Faculty of Built Environment, University of Malaya, 50603 Kuala Lumpur, Malaysia e-mail: firstname.lastname@example.org MS received 20 March 2017; revised 15 July 2017; accepted 3 August 2017; published online 10 March 2018 Abstract. The aim of the present study is to investigate the effects of utilizing different processings of normal rice husk ash (RHA) and black rice husk ash (BRHA) on the mechanical and durability properties of high- strength concrete (HSC). Mechanical and durability properties of HSC were evaluated on concrete mixes containing unground BRHA and RHA and ground BRHA and RHA, their average particles sizes being 165, 85, 67 and 24 lm, respectively. The replacement of ordinary Portland cement with the ashes was adopted at 20%. The results showed that incorporating any form of RHA and BRHA in HSC reduced the slump value. The surface areas of RHA and BRHA, not their carbon content, determined the dosage of superplasticizer needed to achieve a targeted slump value. Concrete with unground and ground RHA incorporated exhibited 30% higher compressive strength while unground BRHA produced 30% lower compressive strength than that of the control concrete. Incorporating unground and ground RHA showed a synergy between filler and pozzolanic effect and had insignificant difference in mechanical and durability properties of the concretes. Meanwhile, incorporating ground BRHA showed a dominant filler effect in the concrete. Overall, the improvement of splitting tensile strength and modulus of elasticity of both RHA and GBRHA concrete showed a similar trend to that of the compressive strength of RHA concrete. The durability of concretes with unground and ground RHA and ground BRHA incorporated showed better performance than that of the control concrete. The material with 20% ground BRHA as partial cement replacement in HSC of Grade 50 could be used without any reduction in the mechanical and durability properties. Use of unground BRHA is not recommended because it did not improve these properties. Keywords. Rice husk ash; high-strength concrete; grinding; particle size; durability; low-cost material. 1. Introduction tonnes of paddy rice was produced annually worldwide  and 20% of that constituted rice husk. Some portions of rice The trend of concrete production nowadays has shifted husk are utilized as fuel sources in boiler for generating from normal to high-strength concrete (HSC), which uti- electricity in rice mill and the rest is dumped and burned in lizes pozzolanic material to improve strength and durability landfills, which can create air pollution. Rice husk has a properties. HSC is defined as a mix having cement content high content of SiO2 in its outer layer . By properly higher than 400 kg/m3 and its compressive strength at burning rice husk and grinding the ash, it can be used as a 28 days of greater than 50 MPa . Rice husk ash (RHA) is mineral admixture in concrete production . A high a pozzolanic material because it contains reactive amor- quality of RHA can be produced by burning rice husk under phous silica through a proper combustion process. One of controlled temperatures of less than 700°C [5, 6]. This type the reasons for increasing research on HSC with RHA of RHA has high amorphous silica, low loss on ignition incorporated is due to the huge availability of rice husk in (LOI) and high SiO2 content. Meanwhile, a low-quality paddy growing countries. In 2013, 745 million metric RHA, the black rice husk ash (BRHA), is a waste product of agricultural industries as a residue of the cyclonic husk furnace at rice mills. The colour of the residue is black due *For correspondence 1
22 Page 2 of 12 Sådhanå (2018) 43:22 to incomplete combustion of rice husk and mostly has beneficial to the concrete industry for applications of RHA lower amorphous silica, higher LOI and lower SiO2 content and BRHA in HSC. than those of normal RHA. BRHA is normally avoided for use in concrete because it does not satisfy the ASTM C 618 requirements such as LOI 2. Material and methodology content of less than 12% and combined proportion of sili- con dioxide (SiO2), aluminium oxide (A12O3) and iron 2.1 Materials oxide (Fe2O3) in the ash of greater than 70%. Nair et al  suggested that BRHA from residue of paddy parboiling OPC used was of type I conforming to ASTM (CEM 42.5) should not be used in producing concrete if its LOI content and its average particle size was 20 lm. Two types of is greater than 20% and SiO2 content is lower than 76%. ashes, BRHA and RHA, and two forms of ashes, unground However, some researchers have shown improvement in and ground, were prepared as partial cement replacement. strength of concrete incorporating BRHA using smaller The BRHA (figure 1a) was received from the rice mills in particle size compared with that of cement and complying Kuala Selangor, Malaysia, denoted as U-BRHA. Mean- with ASTM C 618. Mahmud et al  used BRHA and while, RHA (figure 1b) was produced from combustion in a showed that 15% of BRHA was used as addition to con- ferrocement furnace in the laboratory with peak tempera- crete and it gave optimum strength. When it was used as ture below 700°C and denoted as U-RHA. When rice husk cement replacement, utilizing BRHA as 5% of total binder is heated from 100 to 600°C, the organic matter like cel- could improve mechanical properties. However, Cordiero lulose, lignin, etc. decomposes into carbon . From fig- et al  utilized ultrafine BRHA of 3 lm particle size with ure 1, it can be seen that the colour of BRHA and RHA is LOI of 11.9%. They reported that 20% replacement of black and grey, respectively. The black colour of BRHA is cement with BRHA produced higher mechanical and due to incomplete combustion of rice husk . The BRHA durability properties compared with that of control con- and RHA were ground using a Los Angeles (LA) machine crete. Rego et al  reported that residual RHA with low using 40 steel bars of 10.5 kg as abrasive weight and a amorphous silica content proved to be a suitable mineral rotating drum for 30,000 cycles lasting 16 h. The average addition for cements. Chatveera and Lertwattanaruk  particle size of the U-BRHA was 165 lm, and after used ultrafine BRHA with particle size of less than 12 lm. grinding the average particle size of BRHA was 67 lm, They reported that the compressive strength and durability denoted as G-BRHA (figure 1c). The average particle size properties of concrete were improved when BRHA was of the U-RHA was about 85 lm. After grinding, the aver- used as cement replacement up to 20%. Chopra et al  age particle size of RHA was 24 lm, denoted as G-RHA also mentioned that the inclusion of RHA up to 20% as (figure 1d). The average particle sizes of the G-BRHA were partial replacement to cement in self-compacted concrete larger than that of the G-RHA even after following a sim- improved the strength and durability properties. Mahmud ilar grinding method.  explained that BRHA with particle size of 12 lm The chemical characteristics of BRHA, RHA and OPC could be used to produce HSC of grade 80, especially at 5% were obtained by XRF and LOI analysis. Chemical com- replacement. positions of cement and the two types of RHA are presented The aim of this study is to investigate the effectiveness of in table 1. The chemical compositions of ground RHA and using ground BRHA and RHA on the engineering proper- BRHA are not provided in this paper. There are no sig- ties of HSC. The cost of producing RHA will be increased nificant variations in chemical compositions of the ashes due to the grinding process. Achieving smaller particle size before and after they are ground . It can be seen in this for ashes needs more energy for grinding, and, conse- table that SiO2 content of BRHA and RHA is 63.17% and quently, more cost is needed. As mentioned earlier, in what 85.76%, respectively. LOI percentages of BRHA and RHA most researchers used, the average particle sizes of ashes are 12.8% and 4.05%, respectively. Based on ASTM C 618, were less than that of cement. In this study, the average unground RHA can be classified as a pozzolanic material, particles of ashes used were coarser than those of previous as its silica content is greater than 65% and LOI content is studies, 3 lm  and 12 lm [11, 13]. The average particle lower than 12%. sizes of unground BRHA and RHA were about 165 and The amorphousness of silica in U-BRHA and U-RHA 85 lm, respectively. In addition, the average particle sizes was checked through X-ray diffraction (XRD) analysis. The of ground BRHA and RHA were 67 and 24 lm, respec- XRD data were obtained using a PanAlyticalX’Pert tively. Ordinary Portland cement (OPC) type I was partially diffractometer, operating with Cu radiation replaced with 20% of unground or ground RHA and BRHA (CuKa = 1.54060 Å) and generator settings at 40 mA, by mass of cement in concretes. This paper presents 45 kV. The scanning speed was 20°/min in a 2h range from chemical and physical properties of BRHA and RHA, 50° to 800°. The XRD of U-BRHA and U-RHA in figure 2 compressive strength, splitting tensile strength, modulus of shows that the diffractogram of those ashes has a broad elasticity, permeable porosity and results of rapid chloride hump centred around a 2h angle of 22°, indicating that both permeability test (RCPT). The results of the study would be ashes are amorphous. The crystalline silica on U-BRHA
Sådhanå (2018) 43:22 Page 3 of 12 22 Figure 1. (a) U-BRHA, (b) U-RHA, (c) G-BRHA and (d) G-RHA. 30000 Table 1. Chemical properties of OPC, U-BRHA and U-RHA. Cristobalite 25000 BRHA Chemical composition (%) OPC U-BRHA U-RHA 20000 RHA Magnesium oxide (MgO) 2.06 5.96 0.81 Counts/s Aluminium oxide (Al2O3) 5.60 3.26 0.25 15000 Silicon dioxide (SiO2) 21.28 63.17 85.76 Sulphate (SO3) 2.14 1.14 0.31 10000 Calcium oxide (CaO) 64.64 7.78 0.74 Iron oxide (Fe2O3) 3.38 0.05 1.15 5000 Loss on ignition (LOI) 0.60 12.80 4.05 0 0 20 40 60 80 100 Posion (02 Theta) was possible due to the impurities of the ashes. It was Figure 2. The XRD of (a) BRHA and (b) RHA. collected from an open discharge in the rice mill yard, which may be subjected to some minor contamination from soil ground. Chopra et al  also reported that the silica 3020 V1.04). The particle size distributions of BRHA, was predominantly in amorphous form for incineration RHA and OPC were measured using a laser diffraction temperatures up to 700°C and some cristobalite existed in particle size analyser (Mastersizer S standard Bench – RHA if the combustion exceeded. Malvern instrument) using the dry method. The BET specific surface area was measured using a Fine and coarse aggregates used were mining sand and nitrogen absorption apparatus (MicroActive 2.00-TriStar II crushed granite with a maximum grain size of 4.75 and
22 Page 4 of 12 Sådhanå (2018) 43:22 19 mm, respectively. The specific gravity of the fine and Ws Wd coarse aggregate was 2.84 and 2.66, respectively. permeable porosity ¼ 100% ð1Þ Ws Wb Pipe water that was free from contamination was used in all the mixes. The type of superplasticizer used was poly- where Wb is the buoyant mass of the saturated specimen in carboxylate ether (PCE) with 40% solid content by mass water, Wd is the oven-dry mass of the specimen in air and and was supplied by BASF Sdn. Bhd. Ws is the saturated surface-dry mass of the specimen in air. RCPT was conducted in accordance with ASTM C 1202-97. Concrete cylinders of 100 diameter 9 50 mm 2.2 Mix proportions of concrete mixes height were used for RCPT. Figure 3 shows the test set-up for RCPT. The compressive strength of concrete was Table 2 shows the mix proportions of concrete mixes determined at 1, 3, 7, 28 and 56 days. Meanwhile, the incorporating unground and ground ashes for BRHA and splitting tensile strength of concrete and RCP value were RHA. The control concrete was designed to achieve com- determined at 3, 7, 28 and 56 days. The modulus of elas- pressive strength of 50 MPa at 28 days based on the BRE ticity of concrete was determined at 7 and 28 days. mix design method . Slump values for all the mixes were designed in the range of 100–110 mm. The mixtures contained constant water/binder (w/b) ratio of 0.46 and total 3. Results and discussion binder content of 457 kg/m3. The percentage of cement replacement by ash was 20% . 3.1 Effect of grinding on the physical properties of RHA 2.3 Experimental procedures Table 3 shows some physical properties of OPC, BRHA and RHA. The average particle size of G-RHA is closest to The workability of the fresh concretes was measured using that of OPC; 10% particle sizes of the G-BRHA, U-RHA a slump test based on BS 1881-102. The slump test was and G-RHA are lower than the average particle size of conducted directly before fresh concrete was placed into OPC. Higher concentration of smaller particles in the the moulds. After placement, the specimens were covered cementitious materials will cause higher pozzolanic reac- with polyethylene sheet to prevent water evaporation. The tion . concrete moulds were dismantled after 24 h and the specimens were placed in a water curing tank. Concrete cubes of 100 9 100 9 100 mm3 were casted for com- pressive strength test based on BS 1881-116. For splitting tensile strength and modulus of elasticity, concrete cylinders of 100 mm 9 200 mm and 150 9 300 mm2 dimensions were used based on BS 1881-117 and BS 1881-12, respectively. The permeable porosity was mea- sured as suggested by Safiuddin and Hearn  and the specimens were prepared using the vacuum saturation instead of cold-water or boiling-water saturation tech- niques. The permeable porosity of concrete was calculated based on the concept of weight gain due to permeable porosity and weight loss because of buoyancy. The fol- lowing equation [Eq. (1)] was used to calculate the per- meable porosity of concrete: Figure 3. Rapid chloride permeability test. Table 2. Mix proportions of HSC (kg/m3). Mix ID OPC U-BRHA G-BRHA U-RHA G-BRHA Coarse agg. Fine agg. Water Sp* Control 457 0.0 0.0 0.0 0.0 948 745 210 0.0 U-BRHA 365 92 0 0 0 948 745 210 1.2 G-BRHA 365 0.0 92 0 0 948 745 210 1.5 U-RHA 365 0 0.0 92 0 948 745 210 2.6 G-RHA 365 0 0.0 0 92 948 745 210 2.1 *% of binder and the Sp is specified as the solid mass.
Sådhanå (2018) 43:22 Page 5 of 12 22 Table 3. Physical properties of OPC, BRHA and RHA. Properties OPC U-BRHA G-BRHA U-RHA G-RHA 3 Specific mass (g/cm ) 3.15 1.92 1.98 2.06 2.16 Average particle diameter (lm) 20.085 164.738 66.297 84.382 23.960 Maximum particle diameter below 10% of particle (lm) 3.424 40.395 15.449 13.956 4.146 BET specific surface area (m2/g) 1.060 11.254 19.812 76.195 40.888 Pore volume (cm3/g) 0.004 0.014 0.009 0.160 0.058 Figure 4. Particles in 1.00 k magnification: (a) cement, (b) U-BRHA, (c) G-BRHA, (d) U-RHA and (e) G-RHA. Figure 4 shows the microscopic images of BRHA, RHA the cellular structure of RHA and some fine particles filled and OPC. As can be seen in these figures, the BRHA and the initial pores, resulting in less pores. Habeeb and Mah- RHA grains have porosities while the OPC grains do not mud  mentioned that the surface area of RHA was not have any porosity. FSEM images revealed that RHA is only controlled by average particle sizes but also from the microporous and irregular (figure 4b–e). The average par- RHA’s multi-layered, angular and microporous surface. ticle size of the U-RHA is bigger than that of the G-BRHA Figure 6a shows the particle size distributions of cement, but the surface area of the U-RHA is higher than that of the BRHA and RHA. The ashes are produced under similar G-RHA. As RHA is a porous material, grinding the U-RHA grinding processes but the G-BRHA and the G-RHA have broke the inner pores and reduced both pore volume and its different average particle sizes, which are 66.3 and particle size to 64% and 71%, respectively, and the surface 24.0 lm, respectively. These particle sizes were achieved area of the G-RHA was reduced to 50% of that of the under an optimum grinding time for the G-BRHA and the U-RHA. However, BRHA is less porous compared with G-RHA and beyond that a further reduction of particle size RHA and grinding the U-BRHA increases the surface area required high energy consumption. The difficulty of of the G-BRHA to 50% higher than that of the U-BRHA. grinding fine particles is related to their high strength, low The surface areas of all types of BRHA and RHA are higher capture probability and tendency to agglomerate . Fig- than that of OPC. Figure 5 shows that the fine particles fill ure 6b shows that the fine particles portrayed a unimodal in the porous RHA. A similar observation is reported by particle size distribution while the coarse ones showed a Cordeiro et al , stating that grinding process collapsed bimodal distribution. The unimodal distribution
22 Page 6 of 12 Sådhanå (2018) 43:22 throughout the hydration reaction ; then the mixing water is sufficient for workability of fresh concrete. The workability of a concrete mix is provided by the paste, which fills the voids between aggregates. The paste acts as a lubricant that reduces internal friction between aggregates while increasing workability . However, RHA concrete needed a certain amount of dosage Sp to achieve similar workability to that of fresh control concrete. As can be seen in table 3, BRHA and RHA have higher surface areas and therefore need more water to wet the surface. Therefore, the available mixing water was reduced and it affected the workability of fresh BRHA and RHA concrete. Thus, only mixtures containing BRHA and RHA required additional dosage Sp to achieve the targeted slump value. The G-BRHA mix needed 25% extra Sp than that of the U-BRHA mix. However, the G-RHA mix used 24% less dosage Sp than that of the U-RHA mix to maintain similar workability. A similar result was also found by Rego et al , indicating that incorporating BRHA and RHA in concrete mixtures reduced the slump value of fresh con- Figure 5. Smaller particles fill the pores. crete and the amount of superplasticizer needed was higher to get similar slump to that of fresh control concrete. Figure 7 shows that there is a logarithmic relationship corresponds to the homogeneity of ashes whereas the with strong correlation between specific surface area and bimodal distribution showed their heterogeneous nature dosage of superplasticizer needed. The higher the surface . area of BRHA and RHA, the higher the Sp needed, regardless of the LOI content. This result is in agreement with other researchers , who concluded that the 3.2 Workability of fresh concrete increasing dosage Sp needed in RHA concrete mixtures was related to the surface area of RHA. However, Cordeiro Table 2 shows the dosage of superplasticizer (Sp) used in et al  and Sua-iam and Makul  reported that each mix proportion. In the case of control concrete, it did decreasing slump value of RHA concrete was due to the not require any Sp since its w/b ratio was greater than 0.42. high specific surface area and also the high unburned car- When w/c ratio of OPC concrete is 0.42, all the pores bon content of the RHA. The addition of superplasticizer in within the system are completely filled with water RHA concrete, which is flocculated by cement particles, is 100 5 90 U- BRHA U- BRHA G-BRHA Cumulative passing (%) 80 G-BRHA 4 CEMENT 70 CEMENT U-RHA Volume (%) 60 U-RHA 3 G-RHA 50 G-RHA 40 2 30 20 1 10 0 0 0.01 0.1 1 10 100 1000 10000 0.01 0.1 1 10 100 1000 10000 Particle sizes (mµ) Particle sizes (mµ) (a) (b) Figure 6. The particle size distributions of the cementitious materials (a) based on cumulative passing and (b) based on volume.
Sådhanå (2018) 43:22 Page 7 of 12 22 3.0 Tangapasit et al  reported that the finer particle size of y = 0.7451ln(x) - 0.6557 pozzolan material could improve the packing effect of the 2.5 R² = 0.9929 Dosage of superplasticizer (%) U-RHA material. However, the compressive strengths of U-RHA 2.0 G-RHA concrete at early age are lower than those of the control and G-RHA concrete. This could be because pores of U-RHA 1.5 G-BRHA absorb the superplasticizer, which could retard the hydra- 1.0 U-BRHA tion of cement through the formation of a coating film around hydrated products . The delayed setting time of 0.5 the paste significantly affected the mechanical properties at early ages . As mentioned earlier, the unground RHA 0.0 0 20 40 60 80 100 needed more superplasticizer than the ground RHA so that BET specific surface area (m3/g) the excessive dosage Sp in U-RHA affected its early compressive strength. However, in the case of the Figure 7. Relationship between specific surface area and dosage U-BRHA, its compressive strength is lower than that of of superplasticizer needed for similar workability. control concrete and it is possible that 10% particle size of the U-BRHA is above the average particle size of cement, important for releasing water and, therefore, the released and it does not fill in the ITZ of concrete and thus does not water could lubricate the mixture and create less friction improve the packing density of ITZ. Scrivener et al  among the concrete ingredients. It should be noted that it is pointed out that the particle size of supplementary cemen- very important in RHA concrete production to achieve titious material should be less than the particle size of good workability to ensure appropriate dispersion of the cement in order to improve ITZ of concrete. fine particles and their proper migration into the interface Contrary to the compressive strength of concrete at the transition zone (ITZ) of concrete . early ages, at the end of 28 days and onwards the reaction of concrete incorporating the G-RHA and U-RHA increased compared with that of the G-BRHA, U-BRHA 3.3 Compressive strength and control concrete. From figure 8, it can be seen that the U-RHA and G-RHA concrete exhibited significant Figure 8 shows the compressive strength of BRHA and improvement in compressive strength at later ages. It also RHA concretes relative to that of control concrete up to shows that the effect of retardation on compressive strength 56 days. The 1-day strength of the U-RHA, G-RHA, of the G-RHA concrete is present only at early ages. The G-BRHA and U-BRHA concretes was 94%, 107%, 117% 28-day compressive strengths of the U-RHA, G-RHA, and 60% of control concrete or 17.4, 19.9, 21.8 and G-BRHA and U-BRHA were 122%, 128%, 102% and 68% 11.1 MPa, respectively. It is an interesting phenomenon of control concrete or 64.7, 67.7, 54.1 and 36.2 MPa, that concrete containing G-BRHA exhibited higher com- respectively. The significant improvement in the U-RHA pressive strength at early age compared with that of con- and G-RHA could be related to the pozzolanic reaction of crete containing RHA, which has lower LOI and high silica RHA with Ca(OH)2, which was released from hydration of content. The improvement in strength that occurred in the cement. Therefore, more calcium silicate hydrate (CSH) G-BRHA concrete at early age could be because 10% was produced. This product was deposited in the pore particle sizes of the G-BRHA are below the average par- system, making the cement paste more homogeneous and ticle size of cement. It could fill the void in cement paste denser than the control concrete . and ITZ, which subsequently make the concrete denser. The increase in compressive strength of the U-RHA and G-RHA confirms the synergy of filler and pozzolanic effect. 140 In the case of the G-BRHA concrete, the rate of compres- concrete to that of OPC concrete (%) 130 Synergy pozzolanic and filler effect sive strength gain was decreased, which confirms that the Relative compressive strength of 120 pozzolanic reaction was less. However, the compressive Filler effect 110 strength of the G-BRHA concrete was still higher than that 100 of the control concrete. As can be seen in table 3, although 90 Dilution effect the average particle size of the G-BRHA is three times 80 higher than that of OPC, its 10% particle size was below the 70 60 OPC G-RHA U-RHA average particle size of cement. Its compressive strength 50 U-BRHA G-BRHA gains could be due to the filler effect. Meanwhile, the 40 strength of the U-BRHA concrete was 75% of that of the 0 10 20 30 40 50 60 control concrete, which meant that the U-BRHA concrete Age (days) experienced dilution effect since early age. The U-BRHA Figure 8. Relative compressive strength of BRHA and RHA has low-reactivity pozzolan and high LOI content, and its concrete to that of control concrete. particle size is bigger than that of cement. An inert material
22 Page 8 of 12 Sådhanå (2018) 43:22 having porous structures provides weaker areas in the strength. The G-BRHA concrete showed higher compres- hardened matrix . The large particle size of SCM could sive strength at early age but had less tensile strength than weaken the microstructure  and could have negative that of control concrete. The increase in the rate of strength effect on the concrete. gain of the G-BRHA concrete after 7 days showed that the This information is very useful to the concrete industries, G-BRHA has an amount of reactive amorphous silica even where they can choose the type of RHA and processing to though its existing average particles were 70 lm. It was be used to produce concrete of Grade 50. The use of the reported [35, 36] that RHA particles size in the range of G-RHA and U-RHA in HSC is recommended, but this 10–75 lm had satisfactory pozzolanic behaviour. The increases the cost of concrete production because the rice G-BRHA was less reactive due to its higher LOI content husk has to be burned at controlled temperature in the range and lower SiO2 content compared with those of RHA. In of 600–700°C. As an alternative, the G-BRHA, which does the case of the U-BRHA concrete, its splitting tensile not require specific treatment, could be used as partial strength was lower and it could be due to poor bonding in cement replacement for HSC of Grade 50. the matrix  and also the U-BRHA produced the weakest points in the hardened matrix due to its porous structure . However, even though its improvements in strength 3.4 Splitting tensile strength were lower than that of control concrete, after 7 days the strength of the U-BRHA increased with increasing age, Figure 9 shows the relative splitting tensile strength of which indicated a slow pozzolanic reaction. BRHA and RHA concrete to that of control concrete. The splitting tensile strength of concrete incorporating the U-RHA and G-BRHA improved since the early age. Con- 3.5 Modulus of elasticity crete incorporating G-BRHA showed improvement after 7 days; however, concrete incorporating the U-BRHA Figure 10 shows the result of the modulus of elasticity of showed lower tensile strength than that of control concrete. various RHA concretes. All concretes showed a similar The splitting tensile strength of the U-RHA, G-RHA, trend in the development of the modulus of elasticity, G-BRHA and U-BRHA concrete was 122%, 136%, 118% except for the U-BRHA concrete. The modulus of elasticity and 85% of that of the control concrete at 28 days or 4.6, of the U-BRHA concrete is lower than that of control 5.1, 4.4 and 3.2 MPa, respectively. concrete and this trend is consistent with the development The increasing trend of splitting tensile strength of of the compressive and splitting tensile strength of these BRHA and RHA concretes is similar to that of compressive concretes. At 28 and 56 days, the difference in modulus of strength development. It can be seen from figure 9 that the elasticity of control concrete with that of RHA and the rate of tensile strength gain of the U-RHA concrete G-BRHA concrete is only 5%, which is insignificant. It can decreased before 7 days and the G-RHA concrete increased be concluded that BRHA and RHA do not have significant after 7 days. It shows that the pozzolanic reaction is con- influence on the modulus of elasticity. Since compressive tinuous. Decreasing rate of strength was the result of lack of strengths (at 28 days) of these concretes vary from 45 to calcium hydroxide (CH). Increasing rate of strength gain 60 MPa, they can be referred to as HSC. Thus, the modulus means that large amount of CH was available, which could of elasticity can be predicted using the equation from ACI react with SiO2 and produced CSH and therefore the bond 318-95 for HSC. strength increased. However, improvement in the splitting ACI 318-95  suggests Eq. (2) to relate elastic mod- tensile strength could also be due to the increased bond ulus and compressive strength of concrete: 140 OPC G-RHA 125 Relative splitting tensile strength of BRA 130 U-RHA U-BRHA OPC G-RHA and RHA concrete to that of OPC (%) Relative modulus of elasticity of BRA and G-BRHA 120 U-RHA U-BRHA RHA concrete to that of OPC (%) 120 115 G-BRHA 110 110 100 105 90 100 80 95 90 70 85 60 3 7 28 56 80 Age (days) 0 10 20 30 40 50 60 Age (days) Figure 9. Relative splitting tensile strength of BRA and RHA concrete to that of OPC (%). Figure 10. Development of modulus elasticity of HSC.
Sådhanå (2018) 43:22 Page 9 of 12 22 Table 4. Predicted and measured modulus of elasticity of concrete. Type of Age Equivalent cylinder Measured modulus of Predicted modulus of elasticity Measured Ec/ concrete (days) compressive strength (MPa) elasticity (GPa) from Eq. (2) (GPa) predicted Ec OPC 7 days 35.2 28.6 27.9 0.97 28 days 47.6 32.1 32.4 1.01 U-BRHA 7 days 25.0 26.9 23.5 0.87 28 days 32.6 30.4 26.8 0.88 G-BRHA 7 days 38.7 28.6 29.2 1.02 28 days 48.7 32.1 32.8 1.02 U-RHA 7 days 43.8 30.4 31.5 1.01 28 days 58.2 32.8 35.9 1.09 G-RHA 7 days 44.8 31.1 31.1 1.02 28 days 60.9 33.4 36.7 1.10 *A factor of 0.9 was used to convert cube to cylinder compressive strength. 16.0 Ec ¼ 4:73ðfc Þ1=2 ð2Þ 14.0 where fc is the compressive strength of standard cylinder 12.0 Permeable porosity (%) specimen and Ec is the modulus of elasticity. As can be 10.0 seen in table 4, except for concrete containing the 8.0 U-BRHA, Eq. (2) can give a close estimation compared to 6.0 the experimental values. It should be noted that the value of the modulus of elasticity is an important parameter in 4.0 OPC G-RHA U-RHA U-BRHA G-BRHA designing a structure with regard to deformation. 2.0 0.0 0 10 20 30 40 50 60 3.6 Permeable porosity Age (days) Figure 11 shows the changes of permeable porosity in Figure 11. Permeable porosity of HSC incorporating RHA and control concrete and concretes incorporating RHA and BRHA. BRHA at different ages. The G-RHA concrete had the than 10% and from the permeable porosity point of view, lowest permeable porosities at all ages for 7 and 56 days the G-BRHA concrete can be used as HSC of Grade 50. and its permeable porosity was 4.8% and 2.7%, respec- Figure 12 shows the relationship between permeable tively; this value for control concrete was 5.7% and 4.1%, porosity and compressive strength of concrete with good respectively. The highest permeable porosity was exhibited correlation. The figure clearly shows that improvement of by U-BRHA concrete, which was 5.7% and 4.6%, respec- tively. The lower permeable porosity for the G-RHA, U-RHA and G-BRHA concretes is believed to be due to the 80 hydration process, pozzolanic reaction and filler effect of RHA. 70 Grinding of BRHA and RHA increased their surface 60 Compressive strength (MPa) areas, which improved the capability of SiO2 of BRHA and 50 RHA to react with CaOH from cement hydration. As can be seen in figure 11, permeable porosity of the G-BRHA 40 concrete is lower than that of control concrete. This shows 30 that grinding, as mechanical treatment for low-quality y = -6.1376 x + 113.96 20 RHA, significantly improved its performance in permeable R² = 0.8978 porosity of concrete when compared with the U-BRHA. In 10 the case of the U-RHA and G-RHA, the filler effect and 0 pozzolanic effect synergize each other and reduce the 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 porosity . This resulted in their permeable porosity Permeable porosity (%) being lower than that of the BRHA concrete. Most good concretes have permeable porosity below 10% of its mass Figure 12. Relationship between permeable porosity and com- . The present concretes have permeable porosity of less pressive strength of concrete.
22 Page 10 of 12 Sådhanå (2018) 43:22 1000 4. Conclusions 900 OPC G-RHA U-RHA U-BRHA G-BRHA 800 In this study, black rice husk and grey RHA were ground 700 using the LA abrasion machine. The average particle sizes Charge (C) 600 of BHRA and RHA used were coarser than those previ- 500 ously reported [9, 11, 13]. Fresh, mechanical and durability 400 properties of concrete containing 20% unground and 300 200 ground RHAs were investigated and compared to the 100 properties of control concrete. Based on the test results of 0 this study, the following conclusions can be drawn: 0 10 20 30 40 50 60 Age (days) 1. The surface areas of RHA or BRHA, not their carbon content, determined the dosages Sp required for similar Figure 13. The RCP values of various BRHA and RHA workability compared to the control concrete. concretes. 2. Particles of unground and ground RHA showed syn- ergies between pozzolanic and filler effects in concrete compressive strength is related to the reduction in perme- while ground BRHA acted dominantly as a filler effect. able porosity. A strong correlation of R2 = 0.8978 between On the other side, unground BRHA exhibited a dilution the two parameters was achieved. effect. 3. The effect of grinding of RHA on the mechanical and durability properties of HSC with a w/b of 0.46 is 3.7 Rapid chloride permeability insignificant. 4. RHA can be used as partial cement replacement in the According to ASTM C 1202, concrete having chloride ion form of unground and ground ash due to the insignificant penetrability value in the range of 100–1000°C is catego- difference between unground and ground RHA in the rized as having very low ion penetration. As shown in mechanical and durability properties of HSC. figure 13, all concretes have RCP values of less than 1000 5. The compressive strength of concretes containing 20% C and it indicates that all concretes have the capability to ground BRHA as partial cement replacement attained the resist harmful substances when they are subjected to chlo- values equivalent to that of control concrete after ride penetration. The RCP of the G-RHA, U-RHA, 28 days. The results demonstrated that it is possible to G-BRHA and U-BRHA concrete was 29%, 35%, 59% and develop acceptable ground BRHA concrete with com- 128% of the control concrete at 3 days, respectively. After parable or better strength than that of the control 7 days, RCP value of the G-RHA, U-RHA and G-BRHA concrete using lower cement content. Reducing usage concrete was not much reduced and it exhibited a similar of cement in concrete reduces environment pollution trend regarding the permeable porosity behaviour. At during the cement production. 28 days, the G-RHA, U-RHA, G-BRHA and U-BRHA had 6. After 56 days, the permeable porosity values of all RHA RCP values of 24%, 28%, 52% and 108% of the control concretes are less than 4%, except for unground BRHA concrete, respectively. The U-BRHA concrete showed concrete. This shows that unground BRHA cannot poorer chloride resistance with RCP values of about 700°C improve the microstructures of concrete as well as other but this value was in the range of that of a good concrete. types of RHA and it confirms that unground BRHA is The reduced coulomb values are in agreement with the not recommended for use in HPC of Grade 50. results of other researchers for HSC [40, 41]. RHA reduced 7. The RCP values of concretes containing any type of the value of chloride penetrability in concrete from a low to RHA and ground BRHA were significantly less than that very low ratings from higher to lower replacement levels of the control concrete. This indicates that incorporation and the optimum replacement of cement with RHA for low of RHA significantly improves the durability of HSC. coulomb value is 25% . The high RCP value of the U-BRHA concrete indicated that the high LOI content and coarse particle of BRHA may contribute to the conductivity of the medium . Incorpo- Acknowledgement ration of the G-BRHA as a mineral admixture improved the durability properties of HSC. Test results indicate that The authors would like to thank the Ministry of Science and although the G-BRHA was not as effective as the U-RHA Environment of Malaysia for awarding the IPPP Grant No. and G-RHA, using low energy to grind, preparing G-BRHA PS113/2008B and the UMRG Grant No. UMRG RP018/ samples is relatively easy. It could significantly improve the 2012C to carry out the research on high strength rice husk durability of HSC. Therefore, the G-BRHA can be used as a ash concrete. The authors acknowledge the undergraduate mineral admixture in HSC, especially in rural areas. students: Y W Yee and Y T Yeap, for helping in the
Sådhanå (2018) 43:22 Page 11 of 12 22 concrete laboratory tests. The help of BASF (M) Sdn. Bhd. of the ESCAP/RCTT Third Workshop on Rice Husk Ash in supplying the superplasticizer is highly appreciated. Cements, New Delhi  Marsh B, Teychenne D, Franklin R and Erntroy H 1997 Design of normal concrete mixes. United Kingdom: Con- struction Research Communications Ltd References  Safiuddin M and Hearn N 2005 Comparison of ASTM sat- uration techniques for measuring the permeable porosity of  Phan L T 2002 High-strength concrete at high temperature—an concrete. Cement Concr. Res. 35(5): 1008–1013 overview. In: Proceedings of the 6th International Symposium  Shi C, Wu Y, Riefler C and Wang H 2005 Characteristics on Utilization of High Strength/High Performance Concrete and pozzolanic reactivity of glass powders. Cement Concr.  FAO 2015 Rice market monitor, vol XVIII, issue 1 Res. 35(5): 987–993  Jauberthie R, Rendell F, Tamba S and Cisse I 2000 Origin of  Habeeb G A and Mahmud H B 2010 Study on properties of the pozzolanic effect of rice husks. Constr. Build. Mater. rice husk ash and its use as cement replacement material. 14(8): 419–423 Mater. Res. 13(2): 185–190  Ganesan K, Rajagopal K and Thangavel K 2008 Rice husk  Gosalvitr P, Srinophakun P, Kanchanapiya P and Danwit- ash blended cement: assessment of optimal level of tayakul S 2015 The effects of particle size and content of rice replacement for strength and permeability properties of husk ash from textile wastewater treatment on the properties concrete. Constr. Build. Mater. 22(8): 1675–1683 of Portland cement-base solidification. In: Proceedings of the  Chindaprasirt P, Homwuttiwong S and Jaturapitakkul C 2007 International Conference on Biological, Environment and Strength and water permeability of concrete containing palm Food Engineering (BEFE-2015), May 15–16 oil fuel ash and rice husk–bark ash. Constr. Build. Mater.  Aı̈tcin P C 2001 The ingredients of high-performance con- 21(7): 1492–1499 crete. Concr. Int. 20–21  de Sensale G R 2006 Strength development of concrete with  Mindess S, Young F and Darwin D 2003 Concrete, 2nd ed. rice-husk ash. Cement Concr. Compos. 28(2): 158–160 New Jersey, USA: Prentice-Hall  Nair D G, Jagadish K and Fraaij A 2006 Reactive pozzolanas  Mahmud H B and Bahri S 2014 Mechanical properties of from rice husk ash: an alternative to cement for rural hous- high strength high performance 100 MPa concrete incorpo- ing. Cement Concr. Res. 36(6): 1062–1071 rating rice husk ash. In: Proceedings of the 8th International  Mahmud H B, Majuar E, Zain M F M, Rauf A R A and Beh Conference on Engineering and Technology Research. K B 2003 Feasibility of using black rice husk to produce high Dubai, UAE: Novotel World Trade Centre strength concrete. In: Proceedings of the International  Sua-iam G and Makul N 2013 Utilization of limestone Conference, The Concrete Institute of Australia (CIA), powder to improve the properties of self-compacting con- Brisbane, Australia, pp. 1239–1249 crete incorporating high volumes of untreated rice husk ash  Cordeiro G C, Toledo Filho R D and de Moraes Rego as fine aggregate. Constr. Build. Mater. 38: 455–464 Fairbairn E 2009 Use of ultrafine rice husk ash with high-  Hu J and Stroeven P 2004 Properties of the interfacial tran- carbon content as pozzolan in high performance concrete. sition zone in model concrete. Interface Sci. 12(4): 389–397 Mater. Struct. 42(7): 983–992  Tangpagasit J, Cheerarot R, Jaturapitakkul C and Kiattiko-  Rêgo J, Nepomuceno A, Figueiredo E and Hasparyk N 2015 mol K 2005 Packing effect and pozzolanic reaction of fly ash Microstructure of cement pastes with residual rice husk ash in mortar. Cement Concr. Res. 35(6): 1145–1151 of low amorphous silica content. Constr. Build. Mater. 80:  Heikal M and Aiad I 2008 Influence of delaying addition 56–68 time of superplasticizers on chemical process and properties  Chatveera B and Lertwattanaruk P 2011 Durability of con- of cement pastes. Ceram. Silikaty 52(1): 8 ventional concretes containing black rice husk ash. J. Envi-  Tandırlı E, Akalın Ö and Arca E 2000 Effects of different ron. Manage. 92(1): 59–66 superplasticizers on early strength of concrete. In: Proceed-  Chopra D, Siddique R and Kunal 2015 Strength, perme- ings of the Fifth CANMET/ACI International Conference on ability and microstructure of self-compacting concrete con- Durability of Concrete, Barcelona, Spain taining rice husk ash. Biosyst. Eng. 130: 72–80  Scrivener K L, Crumbie A K and Laugesen P 2004 The  Mahmud H 2010 Properties of high strength concrete interfacial transition zone (ITZ) between cement paste and incorporating black rice husk ash. In: Proceedings of the 2nd aggregate in concrete. Interface Sci. 12(4): 411–421 ASEAN Civil Engineering Conference, Vientiane, Laos  Chowdhury S, Maniar A and Suganya O 2015 Strength  Ramadhansyah Putra J, Mahyun A W, Salwa M Z M, Bakar development in concrete with wood ash blended cement and A, Megat Azmi M J and Mohd Haziman W I 2012 Thermal use of soft computing models to predict strength parameters. analysis and pozzolanic index of rice husk ash at different J. Adv. Res. 6(6): 907–913 grinding time. Procedia Eng. 50: 101–109  Le Thanh Ham K S and Ludwig H M 2012 Synergistic effect  Krishnarao R, Subrahmanyam J and Kumar T J 2001 Studies of rice husk ash and fly ash on properties of self-compacting on the formation of black particles in rice husk silica ash. J. high performance concrete. In: Proceedings of Hipermat Eur. Ceram. Soc. 21(1): 99–104 2012. 3rd International Symposium on Ultra-High Perfor-  Rukzon S, Chindaprasirt P and Mahachai R 2009 Effect of mance Concrete (UHPC) and Nanotechnology for High grinding on chemical and physical properties of rice husk Performance Construction Materials, Kassel University ash. Int. J. Min. Metall. Mater. 16(2): 242–247 Press GmbH  Chopra S, Ahluwalia S and Laxmi S 1981 Technology and  Chindaprasirt P, Kanchanda P, Sathonsaowaphak A and Cao manufacture of rice husk masonry cement. In: Proceedings H 2007 Sulfate resistance of blended cements containing fly
22 Page 12 of 12 Sådhanå (2018) 43:22 ash and rice husk ash. Constr. Build. Mater. 21(6):  Erdem T K and Kırca Ö 2008 Use of binary and ternary 1356–1361 blends in high strength concrete. Constr. Build. Mater. 22(7):  Hwang C L and Chandra S 1997 The use of rice husk ash in 1477–1483 concrete. Norwich, NY: William Andrew Publishing/Noyes,  Neville A M 2008 Properties of concrete, 14th ed. Malaysia: pp. 184–234 CTP-VVP  Mehta P 1979 The chemistry and technology of cements  Saraswathy V and Song H W 2007 Corrosion performance of made from rice husk ash. In: Proceedings of the UNIDO/ rice husk ash blended concrete. Constr. Build. Mater. 21(8): ESCAP/RCTT Workshop on Rice-Husk Ash Cement, Pesha- 1779–1784 war, Pakistan  Nehdi M, Duquette J and El Damatty A 2003 Performance of  A.C. 318 1995 Building code requirements for reinforced rice husk ash produced using a new technology as a mineral concrete. American Concrete Institute admixture in concrete. Cement Concr. Res. 33(8): 1203–1210
You can also read
Next part ... Cancel